The low-temperature catalyzed etching of gallium arsenide with hydrogen chloride Jeffrey L. Dupuie and Erdogan Gulari Department of Chemical Engineering, The University of Michiggn, Ann Arbor, Michigan 48109 (Received 18 September 1991; accepted for publication 10 January 1992) A heated tungsten filament has been used to catalyze the gas phase etching of gallium arsenide with hydrogen chloride at a substrate temperature of 563 K. Rapid etch rates, between 1 and 3 microns per minute, were obtained in a pure hydrogen chloride ambient in the pressure range of 3.3 to 20.0 Pascal. Low flow rates of hydrogen quenched the etching reaction, and resulted in degradation of the quality of the etched gallium arsenide surface. Dilution of the hydrogen chloride to 10.5% in helium reduced the etch rate to 63 nanometers per minute. The removal of 83 nm of gallium arsenide with the helium-diluted gas mixture resulted in a specular surface. X-ray photoelectron spectroscopy indicated that the gallium arsenide surface became enriched in gallium after the etch in helium-diluted hydrogen chloride. No tungsten or other metal contamination on the etched gallium arsenide surface was detected by x-ray photoelectron spectroscopy.
BACKGROUND We reported previously that high purity aluminum ni- tride and silicon nitride films could be deposited by low- Development of a dielectric deposition scheme for the pressure chemical vapor deposition (LPCVD) at low sub- fabrication of viable gallium arsenide metal-insulator- strate temperatures through the catalytic action of a heated semiconductor devices will probably include an in situ sur- filament.5’6 In this process, a heated tungsten filament is face pretreatment prior to dielectric deposition due to a used to decompose ammonia. Products from the decompo- high density of semiconductor surface states. These surface sition of ammonia react with either a group III or group IV states effectively pin the Fermi level of gallium arsenide precursor to form the nitride am. Deposition rates in ex- near midgap. A promising pretreatment for such a deposi- cess of 200 nm/min have been achieved without a plasma, tion scheme is exposure of the gallium arsenide surface to and the resultant film quality compares favorably to nitride hydrogen chloride, which has been shown to reduce the deposited with ECR microwave discharges.7-9 To further surface state density and weaken Fermi level pinning.’ the investigation of the use of films deposited by catalyzed Hydrogen chloride has been shown to be effective in LPCVD: as passivation layers and dielectrics for III-V removing oxygen and carbon contamination from the sur- compound semiconductors, a hydrogen chloride gas feed face of gallium arsenide prior to homoepitaxial growth by has been added to the reactor system. The hydrogen chlo- molecular beam epitaxy ( MBE)2 and metal-organic mo- ride gas feed will allow the exploration of various gallium lecular beam epitaxy ( MOMBE). Oxide free surfaces arsenide surface pretreatments prior to dielectric film have been prepared by room-temperature exposure of gal- growth. In this paper, results are presented for the etching lium arsenide to hydrogen chloride vapor at pressures of gallium arsenide through the decomposition of hydro- greater than 13 Pa.’ However, carbon contamination at the gen chloride by a heated tungsten filament. This initial epitaxial layer interface increased by a factor of four with study focuses on the effects of the reactor pressure, the the hydrogen chloride exposure. Despite this contamina- diluent gas type, and the diluent gas flow rate on the gal- tion, the epitaxial gallium arsenide layer exhibited oval de- lium arsenide etch rate and surface morphology. fect densities a factor of five lower than the level of defect densities obtained with regular substrate preparation. Hy- EXPERIMENT drogen chloride gas phase etching of gallium arsenide at temperatures in the range of 720 to 920 K prior to ho- The combined chemical vapor deposition and etching moepitaxial gallium arsenide via MOMBE has also re- system consists of a six inch diameter, six way stainless- sulted in improved epitaxial layer properties.3 Smooth sub- steel cross reactor, and has been described in detail strate surfaces were reported for substrates etched to 25 previously.s*6 Semi-insulating (100) gallium arsenide wa- nm; no surface morphological results were reported for fers were pressed by molybdenum clamps against an oxi- deeper etches. Substrates prepared by cleaning in dized silicon wafer which was in turn clamped against a hydrogen/hydrogen chloride mixtures exhibited improved stainless-steel susceptor. The susceptor was heated by two interfacial carrier concentrations, with interfacial carbon 300 W cartridge heaters. A sheathed type K thermocouple concentrations reduced by an order of magnitude com- inserted into a thermowell drilled near the surface of the pared to thermal etching. Improved carrier concentrations susceptor was used to monitor the susceptor temperature. have also been achieved for gallium arsenide epitaxial The wafer temperature was calibrated under reaction con- growth by MBE through the use of a hydrogen radical ditions with a type C thermocouple clamped to the surface pretreatment created by an electron cyclotron resonance of the wafer. The tungsten filament temperature was mea- (ECR) microwave plasma.4 sured with a pyrometer, and was set to 2020 K. To confirm
4030 J. Appl. Phys. 71 (8), 15 April 1992 0021-8979/92/084030-04$04.00 @ 1992 American Institute of Physics 4030 TABLE I. Reactor etching parameters and etch rates for the catalyzed 1QUARTZ ROD gas phase etching of gallium arsenide with hydrogen chloride.
I TUNGSTEN Substrate Pressure HCI flow Hz flow He ilow Etch rate FILAMENT Sample temp. (K) (Pa) (seem) (seem) (seem) (nm/min) 4G 563 20 19.2 0 0 1820 STAINLESS 4F 563 6.7 19.2 0 0 3060 STEEL SF 563 3.3 12.7 0 0 1720 SUPPORT 4L 563 6.7 STRUCTURE 19.2 4.3 0 630 5B 563 6.7 19.2 10.4 0 0 SC 563 6.7 4.3 0 36.5 63
1 POSITIONING J~REWS face. Analogous to the decomposition of other molecules on hot filaments, to the low-pressure hydrogen chloride de- composition rate to form chloride atoms may be linearly rh proportional to the hydrogen chloride pressure at the high POWER FEEDTHROUGHS filament temperatures used in this study. At higher reactor pressures, however, radical recombination in the gas phase FIG. 1. Heated tungsten filament unit. can be expected to lower the flux of chlorine atoms arriving at the gallium arsenide surface. Thus, the gallium arsenide etch rate can be expected to exhibit a maximum with re- the pyrometer readings, the average tungsten filament re- spect to the reactor pressure. The feed rate of hydrogen sistivity was measured and gave results which confirmed chloride was limited to 12.7 seem at 3.3 Pa due to the the pyrometer measurements to within 50 K. lower pumping speed of the vacuum pump at low reactor The tungsten filament unit consisted of 93 cm of 0.25 pressures. Calculations based upon the assumption of fully mm diameter tungsten wire wrapped around 13 mm diam- chlorinated reaction products indicated that less than five eter quartz support rods, as depicted in Fig. 1. The quartz percent of the hydrogen chloride was consumed by the rods were notched to evenly distribute the wound filament. etching reaction, so the decreased feed rate at 3.3 Pa Additional notches in the quartz rods and the stainless- should not appreciably affect the gallium arsenide etch steel supports allowed flexible assembly of the tungsten rate. The extremely rapid etch rates of 1 and 3 ,um/min are filament unit. Stainless-steel sleeves provided connections comparable ,to those reported for hot jet gas etching of to the power feedthroughs. The position of the tungsten gallium arsenide with chlorine. “,12 filament unit could be adjusted by positioning screws. As in Figure 2 shows the surface morphology and the isoto- previous thin nitride film depositions, the unit was located pic nature of the etched gallium arsenide surface at a re- 4 cm from the wafer surface. actor pressure of 6.7 Pa. Under no conditions was aniso- The gallium arsenide was masked with a sputtered film tropic etching observed, as has been reported for of silicon dioxide 140 nm thick. The silicon dioxide was downstream ECR microwave plasma chlorine radical patterned by conventional ultraviolet lithography followed etching.13 Brief etches, less than 1 min, under these condi- by wet etching in a buffered hydrofluoric acid solution. tions yielded smooth surfaces as determined by Nomarski Prior to etching in hydrogen chloride, the substrates were and visual inspection, but scanning electron microscope degreased in the solvent sequence trichloroethane, acetone, (SEM) photographs showed a surface morphology com- and methanol. After a rinse in deionized water, the gallium parable to Fig. 2. The surface of gallium arsenide etched at arsenide surface oxide layer was etched in a 1: 1 solution of 3.3 Pa exhibited similar characteristics to those shown in hydrochloric acid (37%) in deionized water. The sub- Fig. 2. Figure 3 shows the surface morphology obtained at strates were then dried in nitrogen and loaded immediately a reactor pressure of 20 Pa. Facets roughly triangular in into the reactor. The gases employed for etching were shape were observed for etches at pressures higher than 6.7 99.999% helium, 99.999% hydrogen, and 99.997% hydro- Pa. gen chloride. The gallium arsenide etched feature depths Hydrogen was added to the gas mixture to decrease the were measured with a scanning profilometer. gallium arsenide etch rate to a more controllable value for surface pretreatment prior to dielectric deposition. The etch rate dependence on the hydrogen flow rate is listed in RESULTS AND DISCUSSIONS Table I. Low flow rates of hydrogen significantly reduced Table I lists the etch rate of gallium arsenide as a the etch rate. The etch of gallium arsenide was completely function of the reactor pressure for a pure hydrogen chlo- quenched upon the addition of 10.4 seem of hydrogen. The ride feed of 19.2 seem at a temperature of 563 K. The run addition of hydrogen resulted in the degradation of the to run variation in the etch rates was typically limited to etched gallium arsenide surface morphology, as shown in less than ten percent. The etch rate experienced a maxi- Fig. 4. This morphology is very similar to the rough sur- mum at 6.7 Pa. The etch rate is expected to be dependent face morphology reported previously,*4 and observed in on the flux of chlorine atoms to the gallium arsenide sur- our laboratory for the thermal reaction of hydrogen chlo-
4031 J. Appl. Phys., Vol. 71, No. 8, 15 April 1992 J. L. Dupuie and E. Gularl 4031 FIG. 3. Hot filament catalyzed gallium arsenide etched surface. HCl flow = 19.2 seem, pressure = 20 Pa, substrate temperature = 563 K. Note the triangular shaped facets.
ing results.‘5’16 At the temperature used in this study, the major gas phase products from gallium arsenide etching were As, for a five percent mixture of chlorine in helium at 10 - 4 Pa,” and AsCl for pure chlorine gas at 3 X 10 - 2 Pa.16 Temperature programed desorption studies of a GaAs surface exposed to atomic hydrogen, created by a hot tungsten ribbon, have revealed that both hydrogen and arsine desorbed under appropriate atomic hydrogen exposures.*’ No gallium hydride species were observed to desorb, indicating that changes in the GaAs surface stoi- chiometry could occur with atomic hydrogen exposure. Hydrogen desorption occurred at temperatures up to ap- proximately 660 K. Under the conditions employed in this work, atomic hydrogen may exhibit a pressure dependent interaction with surface arsenic sites to prevent the forma- tion of volatile arsenic chlorides, and thus alter the reac- tion mechanism and the surface morphology. The rapid atentuation of the etch rate with increased hydrogen flow suggests that homogeneous or heterogeneous radical re- combination, or the preferential adsorption and reaction of hydrogen on the heated filament limit the etching process.
FIG. 2. Hot filament catalyzed gallium arsenide etched surface. HCI flow = 19.2 seem, pressure = 6.7 Pa, substrate temperature = 563 K (a) and (b) surface morphology, 60” from surface normal. (c) 90” from normal. Note the isotropic nature of the catalyzed etch.
ride with gallium arsenide at higher temperatures (750 to 920 K). These results indicate a possible similarity in the etching mechanism between these two techniques, and also indicate that atomic or molecular hydrogen may induce surface roughness for gas phase chlorine-based gallium ar- senide etches. The etched gallium arsenide surface morphology is ex- pected to depend on the etching mechanism. Mass spec- PIG. 4. Hot filament catalyzed gallium arsenide etched surface morphol- troscopy investigations of the kinetic and products of pure ogy with hydrogen dilution. HZ tlow = 4.3 seem, HCl flow = 19.2 seem, chlorine etching of gallium arsenide have yielded conflict- pressure = 6.7 Pa, substrate temperature = 563 K.
4032 J. Appl. Phys., Vol. 71, No. 8, 15 April 1992 J. L. Dupuie and E. Gulari 4032 tungstenwith hydrogenchloride through a differentmech- anism is a possibility. No measurable change in the resis- tance of the tungsten filament was observed during the course of several runs, indicating minimal attack by hydro- gen chloride on the filament. We might expect, however, a small tungsten contamination of the gallium arsenide sur- face not measurable by XPS from a reaction mechanism involving atomic chlorine attack on the cooler portion of the heated filament in contact with the cooler tungsten filament unit supporting rods.
A hot tungsten filament has been shown to effectively FIG. 5. Hot filament catalyzed gallium arsenide etched surface mrophol- catalyze the etching of gallium arsenide at a substrate tem- ogy with helium dilution. He flow = 36.5 seem, HCI flow = 4.3 seem, perature of 563 K through the dissociation of hydrogen pressure = 6.7 Pa, substrate temperature = 563 K. chloride. Rapid etch rates between 1 and 3 ,um/min were obtained in a pure hydrogen chloride ambient. The addi- tion of small flow rates of hydrogen quenched the etching The unsuitability of hydrogen as a diluent for the cat- reaction and contributed to degradation in the galium ar- alyzed gallium arsenide etching process prompted the in- senide surface morphology. Diluting the hydrogen chloride vestigation of helium as an inert gas diluent to assist in in helium resulted in more feasible etch rates for gallium reducing the galluim arsenide etch rate. Figure 5 shows the arsenide pretreatment prior to dielectric deposition, and gallium arsenide surface after the removal of 83 nm for a also resulted in specular etched galium arsenide surfaces mixture of 10.5% HCl in helium at a flow rate of 40.8 seem for short etching times. The hot filament enhanced gallium and a reactor pressure of 6.7 Pa. The etch rate under these arsenide etching method might provide a feasible gallium conditions was 63 nm/min. The gallium arsenide surface arsenide surface cleaning step prior to dielectric film dep- under these conditions appeared smooth under visual, osition. Thin nitride film depositions can be performed im- Nomarski, and SEM inspection. Higher magnification mediately subsequent to the cleaning/etching procedure SEM inspection of the surface revealed a slight surface merely by gas feed switching from the etching gas mixture texture that could not be resolved. Etches for longer times to the film growth gases. ( > 5 min) under these conditions resulted in moderate roughening of the gallium arsenide surface, with the ap- pearance of hemispherical features possessing a character- ‘H. Hasegawa, H. Ishii, T. Sawada, T. Saitoh, S. Konishi, Y. Lui, and H. istic lateral dimension of 100 nm. Ohno, J. Vat. Sci. Technol. B 6, 1184 (1988). The surface composition of the etched surface illus- ‘J. P. Contour, H. Massies, A. Saletes, M. Outrequin, F. Simondet, and trated in Fig. 5 was investigated by x-ray photoelectron J. F. Rochette, J. Vat. Sci. Technol. B 5, 730 (1987). ‘J. Saito, K. Nanbu, T. Ishikawa, and K. Kondo, J. Cryst. Growth 95, spectroscopy (XPS). No contamination from the reactor 322 (1989). wetted materials iron, copper, molybdenum, and tungsten 4S. Sugata, A. Takamori, N. Takado, K. Asakawa, E. Miyauchi, and H. was observed. Also absent from the etched surface was Hashimoto, J. Vat. Sci. Technol. B 5, 1087 (1988). chlorine. The gallium arsenide surface was oxidized and ‘5. L. Dupuie, F. Terry, and E. Gulari (unpublished). bJ. L. Dupuie, F. Terry, and E. Gulari (unpublished). exhibited carbon contamination, as is expected for sample ‘H. Nomura, H. Nomura, Y. Nakanishi, and Y. Hatanaka, J. Appl. transfer from the reactor chamber to the spectrometer Phys. 69, 990 (1991). chamber. XPS indicated that the surface had become en- *S. Meikle, S. Meikle, Y. Nakanishi, and Y. Hatanaka, J. Appl. Phys. 67, riched in gallium, as was predicted for atomic hydrogen 483 (1990). ‘S. V. Nguyen and K. Albaugh, J. Electrochem. Sot. 136, 2835 (1989). exposure. l7 The measured gallium to arsenic ratio was de- “See, for example, M. Grosman, and D. G. Loffler, J. Catal. 80, 188 termined to be 1.3 from integration of the area of the gal- (1983). lium 2p3 and arsenic 3d photoelectron peaks. “M W Geis, N N. Efremow, and G. A. Lincoln, J. Vat. Sci. Technol. B k, 315 (1986). Substantial tungsten contamination of the gallium ar- ‘*M . W . Geis N. N. Efremow, S. W. Pang, and A. C. Anderson, J. Vat. senide surface was not expected based upon the results of a Sci. Techno;. B 5, 363 (1987). mass spectrometric study of the kinetics of the etching of I3 S Sugata and K. Asakawa, J. Vat. Sci. Technol. B 5, 894 (1987). tungsten with chlorine and atomic chlorine.” The forma- 14S: Dorshchand, L. Daweritz, and H. Berger, Crystal Res. & Technol. 18, 1359 (1983). tion of volatile tungsten chlorides from the reaction of “H. Hou, 2. Zhang, S. Chen, C. Su, W. Yan, and M. Vernon, Appl. tungsten with chlorine is expected to occur only at lower Phys. Lett. 55, 801 (1989). temperatures ( < 1000 K) through an Eley-Rideal mech- 16M Balooch D. R. Olander, and W. J. Siekhaus, J. Vat. Sci. Technol. B anism involving gas phase molecular chlorine or atomic 4, ;94 (198;). “J R. Creighton, J. Vat. Sci. Technol. A 8, 3984 (1990). chlorine. The use of hydrogen chloride precludes a mech- Is&. Balooch, D. S. Fischl, D. R. Olander, and W. J. Siekhaus, J. Elec- anism involving molecular chlorine, although etching of trochem. Sot. 135. 2090 (1988).
4033 J. Appl. Phys., Vol. 71, No. 8, 15 April 1992 J. L. Dupuie and E. Gulari 4033